Click here to load reader
Embed Size (px)
Transcript of StructureandPropertiesofTi/TiBMetal¢â‚¬â€œMatrixComposite ......
Vol. 134 (2018) ACTA PHYSICA POLONICA A No. 3
Proceedings of the International Symposium on Physics of Materials (ISPMA 14), September 10–15, 2017, Prague
Structure and Properties of Ti/TiB Metal–Matrix Composite after Isothermal Multiaxial Forging
S. Zherebtsov∗, M. Ozerov, N. Stepanov and M. Klimova Belgorod State University, Pobeda-85, Belgorod 308015, Russia
Microstructure and mechanical properties of a Ti/TiB metal–matrix composites after multiaxial forging at 850 ◦C to the true strain ε = 5.2 were studied. The composite with 17 vol.% of TiB was produced via spark plasma sintering at 1000 ◦C. Mechanical behavior in terms of aggregated σ-Σε curves during the multiaxial forging demonstrated a pronounced softening following by a steady-like flow stage. The length of TiB whiskers considerably decreased after the first step of the multiaxial forging and then changed insignificantly. The microstructure after the MAF consisted of dislocation-free Ti matrix areas of ≈ 1 µm in diameter and areas with high density of TiB whiskers and high dislocation density. The forging resulted in a considerable increase in ductility of the Ti/TiB metal–matrix composites at room and elevated temperatures without loss in strength.
DOI: 10.12693/APhysPolA.134.695 PACS/topics: 81.20.Ev, 81.40.Gh, 81.40.Lm, 81.70.Bt
1. Introduction One of the attractive way to increase strength-related
properties (strength, hardness, wear resistance, etc.) in titanium and low-alloyed titanium alloys is associated with creating Ti matrix composites with embedded ce- ramic reinforcements by, for example, spark plasma sin- tering (SPS) technology [1–3]. Among various rein- forcements TiB has a close to titanium density, it cre- ates minimal residual stresses and has good crystallo- graphic interface with the Ti matrix [4, 5]. During the SPS the TiB whiskers form as a result of the chemi- cal reaction Ti+TiB2 =Ti+2TiB. However, along with the increased strength, Ti/TiB metal–matrix compos- ites (MMCs) demonstrate poor low-temperature ductil- ity. Mechanical properties of the MMCs can be improved by thermo-mechanical treatment, for example multiple isothermal 2D forging (drawing) [6, 7]. In this paper, mi- crostructure and mechanical properties of 17 vol.% TiB reinforced titanium matrix composites produced by SPS at 1000 ◦C was studied after multiaxial forging at 850 ◦C to ε = 5.2.
2. Materials and procedure Commercial Ti and TiB2 powders of ≈ 25 and ≈ 4 µm
in diameter, respectively, were used as the raw materials. A mixture of 90 wt% Ti and 10 wt% TiB2 (which yields 17 vol.% of TiB during the reaction of Ti + TiB2 → Ti + 2TiB ) was prepared using a Retsch RS 200 vibrating cup mill for 1 h in ethanol at the milling rotation speed of 700 rpm.
Ti/TiB MMC specimens measuring 15 mm in height and 19 mm in diameter were produced using the SPS process under vacuum on a Thermal Technology SPS 10- 3 machine at 1000 ◦C and 40 MPa for 15 min.
∗corresponding author; e-mail: firstname.lastname@example.org
The specimens were subjected to multiaxial forging (MAF) which comprised successive compressions of a sample along three orthogonal directions (this method is also known as “abc” deformation ). The initial strain rate and the true strain per deformation step were 10−3/s and ≈ 0.5, respectively. Compressions were performed on an Instron 300LX testing machine in air at 850 ◦C. Stress–strain curves were recorded for each step. Ten compressions in total were made (the true cumulative strain Σε ≈ 5.2).
A JEOL JEM-2100 transmission electron microscope (TEM) and a Quanta 600 FEG (field-emission-gun) scanning-electron microscope (SEM) were used for mi- crostructure examination of the central region of the specimens. SEM specimens were etched using Kroll’s reagent (95% H2O, 3% HNO3, 2% HF)
Tensile or compression tests were conducted on an In- stron 5882 testing machine at 300 ◦C, 400 ◦C, and 500 ◦C (tensile) or room temperature (compression) at an ini- tial strain rate of 10−3/s. The tensile samples had the gauge measuring 4 mm length and 3 mm×1.5 mm cross- section. The compression specimens were measured as 6 × 4 × 4 mm3. Both the compression and tensile tests were carried out without extensometer mainly due to a very small gage size of the specimens.
3. Results and discussion
In the initial (as-sintered) condition the microstruc- ture of the MMC consisted of TiB whiskers with the average diameter 63±35 nm heterogeneously distributed within the Ti matrix (Fig. 1). In the majority of the mi- crostructure a very high dislocation density was observed most probably due to a large number of TiB particles. Some unreacted TiB2 particles (the volume fraction of 2%) were observed in the microstructure. The residual porosity was ≈ 0.5%.
True stress–true strain curves obtained during multi- axial isothermal forging at 850 ◦C showed an initial hard-
696 S. Zherebtsov, M. Ozerov, N. Stepanov, M. Klimova
Fig. 1. Bright-field TEM image of Ti/TiB MMC mi- crostructure; the inset shows a cross-section of a TiB whisker.
Fig. 2. True stress–true strain curves obtained during the MAF at 850 ◦C.
ening transient, a peak flow stress, and then flow soften- ing during the first compression (Fig. 2). However at late stages (Σe > 3) each stress–strain curve demonstrated a steady-state-like behavior after initial hardening. A no- ticeable difference between the flow stresses in the end of each step and the yield stress of the next step was ob- served. It should be noted also that the flow stress had a trend to decrease with increase of cumulative strain.
Microstructure of the Ti/TiB metal–matrix composite changed considerably as a result of the MAF. A lot of small fragments of TiB were observed in the microstruc- ture of the strained condition (Fig. 3a).
Meanwhile TEM analysis showed that deformation at 850 ◦C to e = 5.2 (10 steps) resulted in the formation of separate areas (1–1.5 µm in diameter) with a much lower dislocation density compared with the neighbor-
Fig. 3. SEM (a) and TEM bright-field (b) images of the Ti/TiB composite after the MAF at 850 ◦C to e = 5.2 (10 steps).
ing fields (Fig. 3b). The estimated dislocation density in these areas was ≈ 2×1012 m−2. The boundaries of some dislocation-free areas can be well-defined. The develop- ment of recovery or recrystallization was more evident in the areas of the Ti matrix with a relatively low den- sity of the TiB whiskers. The greater density of the TiB particles most likely hindered grain boundary movement thereby preserving the microstructure with a high dislo- cation density.
Quantitative analysis showed that the diameter of the whiskers did not noticeably change during the MAF. The apparent length of whiskers decreased considerably, by a factor of ≈ 3, after the first step of the MAF and then remained almost unchanged during further deformation (Fig. 4). Thus, the length-to-diameter aspect ratio of TiB whiskers approached stable value (≈ 10) at the initial stages of deformation and had not changed further.
Structure and Properties of Ti/TiB Metal–Matrix Composite after Isothermal Multiaxial Forging 697
Fig. 4. Apparent length of TiB whiskers in Ti/TiB MMCs during the MAF.
Mechanical behavior of the MMCs obtained in com- pression at room temperature (Fig. 5a) or in tension at 300–500 ◦C (Fig. 5b) showed considerable improvement of ductility of the specimens after the MAF to e = 5.2 (10 steps) at 850 ◦C. The samples of the MMC after the MAF at 850 ◦C demonstrated noticeable compression ductility (≈ 2–3%) at room temperature and similar tensile ductil- ity at 300 ◦C. Meanwhile in the as-sintered condition the tensile specimen of MMC fractured just after the elastic region even at 400 ◦C. Some tensile elongation of the as- sintered composite was recorded only at 500 ◦C. The ulti- mate compression strength of the forged and as-sintered specimens was quite similar at room temperature (2210 and 1960 MPa, respectively) while at elevated temper- atures the specimens after the MAF became noticeably stronger. Quite a large stage of elasticity observed in all conditions of the MMC can be associated with the con- ducting of the tensile test without extensometer; in this case elastic deformation of the tensile machine parts was also included into the overall elastic deformation shown in the stress–strain diagram. In addition the Young mod- ulus of the composite is not too high (≈ 200 GPa [4, 10]) while the yield stress at room temperature almost at- tained 2000 MPa.
After the MAF the ultimate strengths were found to be 765 MPa at 300 ◦C and 540 MPa at 400 ◦C while in the as- sintered condition the maximum attained strengths were 480 MPa at 400 ◦C and 520 MPa at 500 ◦C.
Therefore the results obtained in the current study show a possibility to increase considerably low- temperature ductility without loss in strength of the Ti/TiB MMCs by the multiaxial isothermal forging at 850 ◦C to ε =5.2. The observed improvement of the me- chanical properties is most likely associated with the mi- crostructure developed during the MAF. One of the most obvious effects of plastic deformation at elevated temper- atures on the microstructure of Ti/TiB MMC was a con- siderable (by ≈ 3 times) decrease in the length of the TiB whiskers. This change occurred in the very beginning of
Fig. 5. Stress–strain curves of Ti/TiB MMC in differ- ent conditions tested in compression at room tempera- ture (a) or in tension at elevated temperatures (b).
the MAF (Fig. 4) c